Development of biodegradable polycaprolactone film as an internal fixation material to enhance tendon repair: an in vitro study
© Hu et al.; licensee BioMed Central Ltd. 2013
Received: 23 January 2013
Accepted: 6 August 2013
Published: 19 August 2013
Current tendon repair techniques do not provide sufficient tensile strength at the repair site, and thus early active motion rehabilitation after tendon repair is discouraged. To enhance the post-operative tensile strength, we proposed and tested an internal fixation technique using a polycaprolactone (PCL) biofilm. PCL was chosen for its good biocompatibility, excellent mechanical strength, and an appropriate degradation time scale.
PCL biofilms were prepared by a modified melt-molding/leaching technique, and the physical and mechanical properties and in vitro degradation rate were assessed. The pore size distribution of the biofilm and the paratenon of native tendons were observed using scanning electron microscopy. Next, we determined whether this biofilm could enhance the tensile strength of repaired tendons. We performed tensile tests on rabbit Achilles tendons that were first lacerated and then repaired: 1) using modified Kessler suture combined with running peripheral suture (‘control’ group), or 2) using biofilm to wrap the tendon and then fixation with sutures (‘biofilm’ group). The influence of different repair techniques on tendon tensile strength was evaluated by mechanical testing.
The novel biofilm had supple texture and a smooth surface. The mean thickness of the biofilm was 0.25 mm. The mean porosity of the biofilm was 45.3%. The paratenon of the rabbit Achilles tendon had pores with diameters ranging from 1 to 9 μm, which were similar to the 4–12 μm diameter pores in the biofilm cross-section. The weight loss of the biofilms at 4 weeks was only 0.07%. The molecular weight of PCL biofilms did not change after immersion in phosphate buffered saline for 4 weeks. The failure loads of the biofilm were similar before (48 ± 9 N) and after immersion (47 ± 7 N, P > 0.1). The biofilm group had ~70% higher mean failure loads and 93% higher stiffness compared with the control group.
We proposed and tested an internal fixation technique using a PCL biofilm to enhance tendon repair. Internal fixation with the biofilm followed by standard suturing can significantly increase the tensile strength of tendon repair sites. This technique has the potential to allow active motion rehabilitation during the early post-operative period.
KeywordsTendon injury Internal fixation Biomechanics Microstructure
Tendon injuries are common and surgical repair is often necessary. During the healing process, the most common complication is adhesion formation, which restricts tendon gliding. Historically, repaired flexor tendons were immobilized (fixed in place with an external brace during the first few post-operative weeks) until sufficient healing had occurred to allow motion of the tendon . Thus, adhesion formation inevitably occurred and led to finger dysfunction. During surgical repair, avoidance of tendon trauma and preservation of the anatomic integrity of normally contiguous structures may decrease the adhesion formation [2, 3]. Since about the 1970s, methods of mobilizing repaired tendons have been developed allowing limited passive motion to promote gliding of the tendon during the post-operative period [4–6]. Early passive mobilization might improve tendon healing and enhance tendon gliding and tensile strength at the repair site [7–11], but may also cause the tendon to buckle, roll, or fold up . Over the last three decades, controlled active motion immediately after repair was proposed and tested [13, 14]. Controlled active motion protocols with conventional suture can produce a high percentage of excellent and good outcomes [15, 16]. However, because of the difficulties in controlling the amount of load across the repair site during active motion rehabilitation, this technique is also associated with a high rupture rate [17–19].
The optimal tendon repair technique would not only provide coaptation without gap formation at the repair site, but would also provide sufficient strength to safely allow active mobilization to reduce adhesion formation . Immediate active mobilization of repaired tendons was thought to be the most effective way to restore function, and could decrease or even eliminate adhesions [21–24]. However, in the early period after surgery, the strength of the repair depended completely on the repair materials and suture techniques.
Currently, popular techniques for tendon repair (e.g. the modified Kessler suture plus running peripheral suture) [25–29] do not provide sufficient tensile strength at the repair site to recommend early active mobilization. We hypothesized that wrapping a polycaprolactone (PCL) biofilm around the repair site and fixing it in place would increase the tensile strength of the repaired tendon, creating a stable repair site for post-operative early active mobilization.
PCL was chosen as the material for the internal fixation biofilm because PCL is a non-toxic biodegradable polyester, has a slow degradation rate, and demonstrates excellent mechanical strength and biocompatibility [30–36]. In this study, we examined the material properties of the PCL biofilm to determine whether it could be used to strengthen tendon repairs.
Biofilms were prepared using PCL, and the thickness, porosity, pore size, and in vitro degradation rate were measured. Three aspects of biofilm degradation were investigated: the weight, the molecular weight, and the failure load after 4 weeks in solution.
Biofilm specimen preparation
All chemicals were purchased from Alfa Aesar unless otherwise specified. PCL (molecular weight: 200,000 Da) was purchased from Yisheng New Materials Co., Ltd., Shenzhen, China. Before use, tetrahydrofuran (THF) and N,N-dimethylformamide (DMF) were purified to remove water. Briefly, THF was put in calcium hydride for reflux for 12 h and redistilled, and DMF was stirred in calcium hydride (5% w/v) for 12 h, filtered and then distilled at 20 mmHg. A modified melt-molding/leaching technique was used to prepare the biofilms, using DMF as the porogen. The blending of PCL, THF, and DMF was carried out in a beaker on a magnetic stirrer (HPC07SA-P, APLUS, Union city, CA, USA) operating at 45°C and a stirring speed of 200 rpm. PCL (2 g) was added to 20 ml of THF and mixed for 15 min to prepare a homogeneous solution. Next, 1.7 ml of DMF was added and the solution mixed for another 5 min. The resulting blended solution was placed into a rectangular mold of dimension 140 × 100 × 10 mm, and dried at 25°C until the THF had completely evaporated. To obtain the biofilm, the shaped PCL-DMF blends were immersed in a continuous shaking deionized water bath at 37°C to leach out the DMF. Fresh changes of deionized water were performed every 12 h until the wet specimen reached a constant weight, confirming that all the DMF was removed. Finally, the specimen was lyophilized for 24 h and stored in a dry container until use.
Determination of the porosity and thickness of the biofilm
The porosity of the specimen was measured by Archimedes’ method. First, the specimen was lyophilized to determine the dry weight (W1). Then, the specimen was transferred to a beaker and placed in a vacuum oven at 2 kPa for 15 min, followed by slow injection with water until the specimen was completely immersed. Next, the pressure was gradually restored to atmospheric, and then the saturated specimen was placed in a copper wire basket, suspended in a beaker filled with water, and weighed (W2). The specimen was taken out of the water, any water remaining on its surface was removed with wet gauze, and the specimen was weighed again (W3). The porosity was calculated using the following formula: porosity (%) = [(W3 – W1)/(W3 – W2)] × 100% (n = 12). Thickness was measured using a micrometer (n = 12).
In vitro degradation of the biofilm
The biofilm was cut into 100 mm × 20 mm pieces for in vitro degradation testing. Lyophilized specimens were accurately weighed (W0), and then immersed in phosphate buffered saline (PBS) pH 7.4 in a continuous shaking water bath at 37°C for 4 weeks. The degradation medium of PBS was changed each week. After 4 weeks, the specimens were removed, washed with deionized water, lyophilized, and reweighed (WF). The percent weight loss was calculated as: weight loss % = [(W0 − WF)/W0] × 100% (n = 12). After 4 weeks of degradation, PCL biofilms were dissolved in THF at a concentration of 1 mg/mL and filtered through a 0.2-μm inorganic membrane filter (GE Healthcare, UK). The molecular weight of the biofilm was determined by gel permeation chromatography (GPC apparatus 1525, Waters Co., Milford, MA, USA) (n = 12).
In order to examine the tensile strength, the specimens were fixed in custom-made clamps and mounted in a microcomputer-controlled electronic universal mechanical testing machine (Dual Column Testing System 3369, Instron Co., Norwood, MA, USA). Before testing, both the ends (10 mm) of the specimen were first wrapped with tape and then clipped in the clamps equipped with rubber pads. The initial distance between the fixtures was set at 80 mm. The specimens were distracted at a rate of 5 mm/min until failure. During the testing, if the specimen slipped away from the clamps, or fracture occurred within 10 mm of any clamp, the measurement was considered invalid. Throughout the testing process, fracture occurred in the middle of all specimens and no specimen slipped away from the clamps.
Microstructural characterization of the biofilm and the Achilles tendon outer membrane
Twelve rabbits were euthanized and 1 Achilles tendon was harvested from each. The peeled paratenon of the Achilles tendons were fixed with 2.5% glutaraldehyde, dehydrated by alcohol gradients, soaked in osmium tetroxide, dried and coated with gold, and then the pore size distribution of the tendon outer membrane was observed with field emission scanning electron microscopy (FESEM, Nova NanoSEM 230, FEI Co., Hillsboro, OR, USA) (n = 12). The prepared biofilms were placed in liquid nitrogen for 30 min, broken to pieces, freeze-dried, and evenly sprayed with gold. Finally, the cross-section was observed with FESEM (n = 12).
Establishment of an in vitro model of Achilles tendon repair
Biomechanical testing of the tendon repair model
The repaired tendons were fixed in the universal mechanical testing machine clamps and distracted at a rate of 0.3 mm/min (n = 12). The length of tendon between the clamps was kept constant at 3 cm. The load–displacement curves were simultaneously traced by the testing machine computer. The failure load was defined as the peak load of the repair construct. The stiffness of the repair was calculated as the slope of the linear region of the load–displacement curve. The entire testing process was conducted at a room temperature of 25°C with 70% relative humidity, and the specimens were kept moist with saline spray.
All data obtained are presented as mean ± SD. One-way ANOVA with paired t-tests were performed to detect significant (P < 0.05) effects of the experimental variables.
The biofilm had excellent physical properties
The biofilm degraded slowly in vitro
The biofilm degradation rates and the influence of early degradation on the mechanical properties of the biofilm were observed in vitro. All specimens showed very slow degradation rates after soaking for 4 weeks in PBS. The weight loss of the biofilms was only 0.07 ± 0.005% after 4 weeks.
The molecular weight of the biofilm showed no change from 200,000 Da after 4 weeks soaking in PBS (data not shown). The failure loads of the biofilm were similar before (48 ± 9 N) and after 4 weeks of degradation (47 ± 7 N, P > 0.1). These results were correlated with the minimal weight loss.
The pore size distribution of the PCL biofilm was similar to that of the Achilles tendon paratenon
Internal fixation with the biofilm can significantly increase tensile strength of the tendon repair site
The mean failure load of the control group was 23.5 ± 4.9 N, while that of the biofilm group was 39.6 ± 6.7 N (P < 0.05), an increase of almost 70%. The mean stiffness of the control group was 7.11 ± 1.9 N/mm, while that of the biofilm group was 13.69 ± 5.8 N/mm (P < 0.05), an increase of almost 93%.
Many different repair methods have been explored with the aim of enhancing the tensile strength of repaired tendons [37–40]. For various reasons, however, these methods are not widely used in clinics. For example, Becker et al.  reported a technique involving beveling of the tendon ends and fine compressive suturing. The drawback of this approach is that it causes shortening of the tendon ends. The double loop locking suture technique reported by Lee  and the fish mouth anastomosis method described by Pulvertaft  were able to strengthen the repair; however, normal tendon anatomy is distorted with these methods. The cross-stitch plus mesh sleeve technique described by Silfverskiöld  is time-consuming and technically complicated.
Currently, the modified Kessler suture plus running peripheral suture is the most popular tendon repair technique . However, this suture technique cannot develop enough strength at the suture site, and early active motion may result in a higher incidence of rupture. Therefore, new materials and techniques for increasing the strength of tendon repair sites are needed for hand surgery.
This study presented a biofilm for internal fixation that increased the failure load of in vitro tendon repair by 70% over standard techniques, and, therefore, might allow for the initiation of early active motion rehabilitation.
PCL was chosen because of its desirable material properties, such as good biocompatibility and complete degradation, absorption, and excretion in the body [32, 35, 36, 41, 42]. In a previous study, rat mesenchymal stem cells were able to adhere and proliferate on PCL scaffolds for bone tissue engineering, demonstrating good biocompatibility . In a different study where tritium-labeled PCL (M w: 3,000 Da) was subcutaneously implanted in rats, 92% of the implanted radioactive tracer was excreted from feces and urine by 135 days after implantation . Finally, another study showed that three-dimensional PCL scaffolds (M n 80,000) had no molecular weight change after 6 months in vitro and in vivo, revealing excellent long-term biocompatibility and no adverse host tissue reactions . Very little in vitro degradation of the PCL film prepared (M w 200,000) in the current study was observed after 4 weeks. Therefore, the biofilm would not lose its mechanical properties and would be able to support the injured tendon repair during the early stage of tendon healing. In addition, the high porosity of the biofilms and the size of the pores were similar to those of native tendons, suggesting that the biofilm should not impede tendon nourishment.
While this study indicated that internal fixation with PCL might enhance the strength of the repair after tendon injury and repair, the present research was only an in vitro investigation. Additional in vivo factors involved in tendon healing could be investigated, such as potentially inhibitory effects of wrapping a biofilm around the repair site on the migration of immune cells and fibroblasts to the site. Neutrophils and monocytes infiltrate the repair during the first 3 post-operative days. They play an important role in the clearance of bacteria and debris and are vital for chemotaxis of fibroblasts to the repair site [43–45]. Fibroblasts are the cell type that will eventually rebuild the tendon via the production of collagen [43–45]. Many studies have shown that immune cells and fibroblasts enter the repair site via the surface of the tendon [43–47]. While the pore size of the PCL biofilm is large enough for nutrients and cytokines to infiltrate, it appears to be too small for many of these cell types to gain access to the repair site. Neutrophils are generally 12–15 μm, monocytes are 10–30 μm, and tendon fibroblasts are 20–70 μm in length and 8–20 μm wide. Given that the pores of the biofilm are only 4–12 μm, it appears that the biofilm would inhibit cell infiltration, and thus impede tendon healing. However, many methods could be adopted to enlarge the pore size, such as increasing the DMF concentration while blending the PCL, THF, and DMF. It is also feasible to incorporate sacrificial beads into the biofilms that will degrade, leaving an increased porosity (e.g. use of salt particulate (NaCl) and water-soluble polymer (PEG) as co-porogens ). Further studies should focus on improving the pore size and the porosity of the biofilm, as well as its biocompatibility, degradation, absorption, excretion, and mechanical properties using an in vivo rabbit Achilles tendon repair model.
In this study, we proposed the use of an internal fixation technique and novel material to enhance tendon repair. The biofilms used had high porosity and slow degradation rates in vitro. The pore size distribution of the biofilm was similar to that of the paratenon of rabbit Achilles tendon. Internal fixation with the biofilm followed by standard suture techniques significantly increased the tensile strength of the tendon repair site, and thus might allow early active motion rehabilitation without the risk of rupture. However, in vivo studies are needed to further explore whether the biofilms will enhance the healing properties of repaired tendons.
This work was supported by the China Changsha Municipal Sci-Tech Project (K1101025-31). The authors thank Mr. Li Hengfeng for his technical assistance.
- Peacock E: Fundamental aspects of wound healing relating to the restoration of gliding function after tendon repair. Surg Gynecol Obstet. 1964, 119: 241-250.PubMedGoogle Scholar
- Potenza AD: Effect of associated trauma on healing of divided tendons. J Quant Spectrosc Radiat Transf. 1962, 2: 75-84.Google Scholar
- Potenza AD: Prevention of adhesions to healing digital flexor tendons. JAMA. 1964, 187: 187-191.View ArticlePubMedGoogle Scholar
- Lister GD, Kleinert HE, Kutz JE, Atasoy E: Primary flexor tendon repair followed by immediate controlled mobilization. J Hand Surg Am. 1977, 2: 441-451. 10.1016/S0363-5023(77)80025-7.View ArticlePubMedGoogle Scholar
- Gelberman RH, Menon J, Gonsalves M, Akeson WH: The effects of mobilization on the vascularization of healing flexor tendons in dogs. Clin Orthop Relat Res. 1980, 153: 283-289.PubMedGoogle Scholar
- Gelberman RH, Woo SL, Lothringer K, Akeson WH, Amiel D: Effects of early intermittent passive mobilization on healing canine flexor tendons. J Hand Surg Am. 1982, 7: 170-175. 10.1016/S0363-5023(82)80083-X.View ArticlePubMedGoogle Scholar
- Gelberman RH, Amifl D, Gonsalves M, Woo S, Akeson WH: The influence of protected passive mobilization on the healing of flexor tendons: a biochemical and microangio- graphic study. Hand. 1981, 13: 120-128. 10.1016/S0072-968X(81)80051-4.View ArticlePubMedGoogle Scholar
- Gelberman RH, Manske PR: Factors influencing flexor tendon adhesions. Hand Clin. 1985, 1: 35-42.PubMedGoogle Scholar
- Woo SL, Gelberman RH, Cobb NG, Amiel D, Lothringer K, Akeson WH: The importance of controlled passive mobilization on flexor tendon healing. A biomechanical study. Acta Orthop Scand. 1981, 52: 615-622. 10.3109/17453678108992156.View ArticlePubMedGoogle Scholar
- Takai S, Woo SL, Horibe S, Tung DK, Gelberman RH: The effects of frequency and duration of controlled passive mobilization on tendon healing. J Orthop Res. 1991, 9: 705-713. 10.1002/jor.1100090510.View ArticlePubMedGoogle Scholar
- Boyer MI, Gelberman RH, Burns ME, Dinopoulos H, Hofem R, Silva MJ: Intrasynovial flexor tendon repair. An experimental study comparing low and high levels of in vivo force during rehabilitation in canines. J Bone Joint Surg Am. 2001, 83: 891-899.PubMedGoogle Scholar
- Manske P: Flexor tendon healing. J Hand Surg Br. 1988, 13: 237-245. 10.1016/0266-7681(88)90077-0.View ArticlePubMedGoogle Scholar
- Cullen K, Tolhurst P, Lang D, Page RE: Flexor tendon repair in zone II followed by controlled active motion. J Hand Surg Br. 1989, 14: 392-395. 10.1016/0266-7681(89)90153-8.View ArticlePubMedGoogle Scholar
- Matthews JP: Early mobilization after tendon repair. J Hand Surg Br. 1989, 14: 363-367.View ArticlePubMedGoogle Scholar
- Elliot D, Moiemen NS, Flemming AFS, Harris SB, Foster AJ: The rupture rate of acute flexor tendon repairs mobilized by the controlled active regimen. J Hand Surg Br. 1994, 19: 607-612.View ArticlePubMedGoogle Scholar
- Evans RB: Rehabilitation techniques for applying immediate active tension to zone I and II flexor tendon repairs. Tech Hand Up Extrem Surg. 1997, 1: 286-296. 10.1097/00130911-199712000-00010.View ArticlePubMedGoogle Scholar
- Silfverskiold KL, Anderson CH: Two new methods of tendon repair: an in vitro evaluation of tensile strength and gap formation. J Hand Surg Am. 1993, 18: 58-65. 10.1016/0363-5023(93)90246-Y.View ArticlePubMedGoogle Scholar
- Greenwald D, Shumway S, Allen C, Mass D: Dynamic analysis of profundus tendon function. J Hand Surg Am. 1994, 19: 626-635. 10.1016/0363-5023(94)90272-0.View ArticlePubMedGoogle Scholar
- Schuind F, Garcia Elias M, Cooney WP, An KN: Flexor tendon forces: in vivo measurements. J Hand Surg Am. 1992, 17: 291-298. 10.1016/0363-5023(92)90408-H.View ArticlePubMedGoogle Scholar
- Diao E, Hariharan JS, Soejima O, Lotz JC: Effect of peripheral suture depth on strength of tendon repairs. J Hand Surg Am. 1996, 21: 234-239. 10.1016/S0363-5023(96)80106-7.View ArticlePubMedGoogle Scholar
- Tang JB, Wang B, Chen F, Pan CZ, Xie RG: Biomechanical evaluation of flexor tendon repair techniques. Clin Orthop Relat Res. 2001, 386: 252-259.View ArticlePubMedGoogle Scholar
- Momeni A, Grauel E, Chang J: Complications after flexor tendon injuries. Hand Clin. 2010, 26: 179-189. 10.1016/j.hcl.2009.11.004.View ArticlePubMedGoogle Scholar
- Graf V, Papaloizos , Borisch N, Della Santa D: Interest in early active controlled mobilization and flexion following flexor tendon repair in zone 2. Chir Main. 2001, 20: 458-465. 10.1016/S1297-3203(01)00072-5.View ArticlePubMedGoogle Scholar
- Branford OA, Lee DA, Bader DL, Grobbelaar AO: The mechanics of flexor tendon adhesions. J Hand Surg Eur Vol. 2012, 37: 555-563. 10.1177/1753193411432675.View ArticlePubMedGoogle Scholar
- Winters SC, Seiler JG, Woo SL, Gelberman RH: Suture methods for flexor tendon repair. A biomechanical analysis during the first six weeks following repair. Ann Chir Main Memb Super. 1997, 16: 229-234. 10.1016/S0753-9053(97)80006-3.View ArticlePubMedGoogle Scholar
- Tsuge K, Ikuta Y, Matsuishi Y: Intra-tendinous tendon suture in the hand–a new technique. Hand. 1975, 7: 250-255. 10.1016/0072-968X(75)90062-5.View ArticlePubMedGoogle Scholar
- Ketchum LD: Suture materials and suture techniques used in tendon repair. Hand Clin. 1985, 1: 43-53.PubMedGoogle Scholar
- Strickland JW: Flexor tendon repair. Hand Clin. 1985, 1: 55-68.PubMedGoogle Scholar
- Kessler I: The“grasping” technique for tendon repair. Hand. 1973, 5: 253-255. 10.1016/0072-968X(73)90038-7.View ArticlePubMedGoogle Scholar
- Sun H, Mei L, Song C, Cui X, Wang P: The in vivo degradation, absorption and excretion of PCL-based implant. Biomaterials. 2006, 27: 1735-1740. 10.1016/j.biomaterials.2005.09.019.View ArticlePubMedGoogle Scholar
- Lin HM, Lin YH, Hsu FY: Preparation and characterization of mesoporous bioactive glass/polycaprolactone nanofibrous matrix for bone tissues engineering. J Mater Sci Mater Med. 2012, 23: 2619-2630. 10.1007/s10856-012-4734-z.View ArticlePubMedGoogle Scholar
- Muhammad KB, Abas WA, Kim KH, Pingguan-Murphy B, Zain NM, Akram H: In vitro comparative study of white and dark polycaprolactone trifumarate in situ cross-linkable scaffolds seeded with rat bone marrow stromal cells. Clinics. 2012, 67: 629-638. 10.6061/clinics/2012(06)14.View ArticlePubMedPubMed CentralGoogle Scholar
- Zheng M, Librizzi D, Kilic A, Liu Y, Renz H, Merkel OM, Kissel T: Enhancing in vivo circulation and siRNA delivery with biodegradable polyethylenimine-graft- polycaprolactone-block-poly(ethylene glycol) copolymers. Biomaterials. 2012, 33: 6551-6558. 10.1016/j.biomaterials.2012.05.055.View ArticlePubMedGoogle Scholar
- Peng YJ, Lu YT, Liu KS, Liu SJ, FAN L, Huang WC: Biodegradable balloon-expandable self-locking polycaprolactone stents as buckling explants for the treatment of retinal detachment: an in vitro and in vivo study. J Biomed Mater Res A. 2013, 101: 167-175.View ArticlePubMedGoogle Scholar
- Lam CX, Hutmacher DW, Schantz JT, Woodruff MA, Teoh SH: Evaluation of polycaprol- actone scaffold degradation for 6 months in vitro and in vivo. J Biomed Mater Res A. 2009, 90: 906-919.View ArticlePubMedGoogle Scholar
- Liu L, Wang Y, Guo S, Wang Z, Wang W: Porous polycaprolactone/nanohydroxyapatite tissue engineering scaffolds fabricated by combining NaCl and PEG as co-porogens: structure, property, and chondrocyte-scaffold interaction in vitro. J Biomed Mater Res B Appl Biomater. 2012, 100: 956-966.View ArticlePubMedGoogle Scholar
- Becker H, Orak F, Duponselle E: Early active motion following a beveled technique of flexor tendon repair: report on fifty cases. J Hand Surg Am. 1979, 4: 454-460. 10.1016/S0363-5023(79)80043-X.View ArticlePubMedGoogle Scholar
- Lee H: Double loop locking suture: technique of tendon repair for early active mobilization. Part II: Clinical experience. J Hand Surg Am. 1990, 15: 953-958. 10.1016/0363-5023(90)90022-J.View ArticlePubMedGoogle Scholar
- Pulvertaft RG: Suture materials and tendon junctures. Am J Surg. 1965, 109: 346-352. 10.1016/S0002-9610(65)80083-6.View ArticlePubMedGoogle Scholar
- Silfverskiöld KL, Andersson CH: Two new methods of tendon repair: anin vitro evaluation of tensile strength and gap formation. J Hand Surg Am. 1993, 18: 58-65. 10.1016/0363-5023(93)90246-Y.View ArticlePubMedGoogle Scholar
- Middleton JC, Tipton AJ: Synthetic biodegradable polymers as orthopedic devices. Biomaterials. 2000, 21: 2335-2346. 10.1016/S0142-9612(00)00101-0.View ArticlePubMedGoogle Scholar
- Woodruff MA, Hutmacher DW: The return of a forgotten polymer-polycaprolactone in the 21st century. Prog Polym Sci. 2011, 35: 1217-1256.View ArticleGoogle Scholar
- Strickland JW: The scientific basis for advances in flexor tendon surgery. J Hand Ther. 2005, 18: 94-110. 10.1197/j.jht.2005.01.013. quiz 111View ArticlePubMedGoogle Scholar
- Griffin M, Hindocha S, Jordan D, Saleh M, Saleh M, Khan W: An overview of the management of flexor tendon injuries. Open Orthop J. 2012, 6: 28-35. 10.2174/1874325001206010028.View ArticlePubMedPubMed CentralGoogle Scholar
- Tillman LJ, Chasan NP: Properties of dense connective tissue and wound healing. Management of common musculoskeletal disorders: physical therapy principles and methods. Edited by: Hertling D, Kessler RM. 1996, Philadelphia: Lippincott, 8-21.Google Scholar
- Potenza AD: Critical evaluation of flexor-tendon healing and adhesion formation within artificial digital sheaths. J Bone Joint Surg Am. 1963, 5: 1217-1233.Google Scholar
- Gelberman RH, Vandeberg JS, Manske PR, Akeson H: The early stages of flexor tendon healing: morphologic study of the first fourteen days. J Hand Surg Am. 1985, 10: 776-784. 10.1016/S0363-5023(85)80151-9.View ArticlePubMedGoogle Scholar
- The pre-publication history for this paper can be accessed here:http://www.biomedcentral.com/1471-2474/14/246/prepub
This article is published under license to BioMed Central Ltd. This is an Open Access article distributed under the terms of the Creative Commons Attribution License (http://creativecommons.org/licenses/by/2.0), which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.